IIIE SECTION A MANUFACTURING TECHNOLOGY NOTES 6.investment casting
This process is also called as lost wax process or precision
Castings obtained by this process have very close
tolerances of the order of +/- 0.005mm.Generally this
process is used to produce small and intricate parts.This
process does not need a parting line or any form of split
Casts can be made of the wax model itself, the direct method;
Or of a wax copy of a model that need not be of wax, the indirect
The following steps are for the indirect process which can
take two days to one week to complete.
1.Produce a master pattern :
An artist or mould maker creats an original pattern from
Wax, Wood, steel, or other materials.
2.Mould making :
A mould known as the master die, is made of the master
pattern. The master pattern may be made from a low-
melting-point metal, steel, or wood. If a steel pattern was
created then a low-melting-point metal may be cast directly
from the master pattern. Rubber moulds can also be cast
directly from the master pattern. The first step may also be
skipped if the master die is machined directly into steel.
3. Produce the wax patterns:
Although called a wax pattern, pattern materials also include
plastic and frozen mercury. Wax patterns may be
produced in one of two ways:
(a) The wax is poured into the mold and swished around
until an even coating, usually about 3 mm (0.12 in) thick,
covers the inner surface of the mould. This is repeated until
the desired thickness is reached.
(b) Another method is filling the entire mould with molten
wax, and let it cool, until a desired thickness has set on the
surface of the mould. After this the rest of the wax is poured
out again, the mould is turned upside down and the wax
layer is left to cool and harden. With this method it is more
difficult to control the overall thickness of the wax layer
4, Assemble the wax patterns:
The wax pattern is then removed from the mould. Depending
on the application multiple wax patterns may be created so
that they can all be cast at once. In other applications,
multiple different wax patterns may be created and then
assembled into one complex pattern. In the first case the
multiple patterns are attached to a wax sprue, with the result
known as a pattern cluster, or tree; as many as several
hundred patterns may be assembled into a tree. Foundries
often use registration marks to indicate exactly where they
go. The wax patterns are attached to the
sprue or each other by means of a heated metal tool. The
wax pattern may also be chased, which means the parting
line or flashing are rubbed out using the heated metal tool.
Finally it is dressed, which means any other imperfections
are addressed so that the wax now looks like the finished
The ceramic mould, known as the investment, is produced
by three repeating steps: coating, stuccoing, and hardening.
The first step involves dipping the cluster into a slurry of fine
refractory material and then letting any excess drain off, so a
uniform surface is produced. This fine material is used first to
give a smooth surface finish and reproduce fine details.
In the second step, the cluster is stuccoed with a coarse
ceramic particle, by dipping it into a fluidised bed, placing it
in a rainfall-sander, or by applying by hand.Finally, the
coating is allowed to harden.
These steps are repeated until the investment is the required
thickness, which is usually 5 to 15 mm .Note that the first
coatings are known as prime coats. An alternative to multiple
dips is to place the cluster upside-down in a flask and then
liquid investment material is poured into the flask. The flask
is then vibrated to allow entrapped air to escape and help
the investment material fill in all of the details.
Common refractory materials used to create the investments
are: silica, zircon, various aluminium silicates, and alumina.
Silica is usually used in the fused silica form, but sometimes
quartz is used because it is less expensive. Aluminium
silicates are a mixture of alumina and silica, where
commonly used mixtures have an alumina content from 42
to 72%; at 72% alumina the compound is known as mullite.
During the primary coat(s), zircon-based refractories are
commonly used, because zirconium is less likely to react
with the molten metal. Chamotte is another refractory
material that has been used Prior to silica, a mixture of
plaster and ground up old molds (chamotte) was used
The binders used to hold the refractory material in place
include: ethyl silicate (alcohol-based and chemically set),
colloidal silica (water-based, also known as silica sol, set by
drying), sodium silicate, and a hybrid of these controlled for
pH and viscosity.
The investment is then allowed to completely dry, which can
take 16 to 48 hours. Drying can be enhanced by applying a
vacuum or minimizing the environmental humidity. It is then
turned upside-down and placed in a furnace or autoclave to
melt out and/or vaporize the wax. Most shell failures occur at
this point because the waxes used have a thermal
expansion coefficient that is much greater than the
investment material surrounding it, so as the wax is heated it
expands and induces great stresses. In order to minimize
these stresses the wax is heated as rapidly as possible so
that the surface of the wax can melt into the surface of the
investment or run out of the mold, which makes room for the
rest of the wax to expand. In certain situations holes may be
drilled into the mold beforehand to help reduce these
stresses. Any wax that runs out of the mold is usually
recovered and reused.
7.Burnout & preheating:
The mold is then subjected to a burnout, which heats the
mold between 870 °C and 1095 °C to remove any moisture
and residual wax, and to sinter the mold. Sometimes this
heating is also used as the preheat, but other times the mold
is allowed to cool so that it can be tested. If any cracks are
found they can be repaired with ceramic slurry or special
The mold is preheated to allow the metal to stay
liquid longer to fill any details and to increase dimensional
accuracy, because the mold and casting cool together.
The investment mold is then placed cup-upwards into a tub
filled with sand. The metal may be gravity poured, but if
there are thin sections in the mold it may be filled by
applying positive air pressure, vacuum cast, tilt cast,
pressure assisted pouring, or centrifugal cast
The shell is hammered, media blasted, vibrated, waterjeted,
or chemically dissolved (sometimes with liquid nitrogen) to
release the casting. The sprue is cut off and recycled. The
casting may then be cleaned up to remove signs of the
casting process, usually by grinding.
1. High dimensional accuracy( +/- 0.08)
2. Very smooth surface of the casting. ( 0.015 – 0.025 rms
value)without parting line, can be easily obtained.
3. Suitable for both high and low melting point alloys,
since the ceramic material can be selected to have the
appropriate refractory properties. And bonded with any
desired agent to give the required strength and
4. It is a flexible process and can reproduce surface details
and dimensions with precision, especially for high
melting point alloys.
5. Undercuts and other shapes which would not aloe the
withdrawal of a normal pattern are easily provided. No
cores or loosed pcs are reqd.
6. Machining of intricate parts can be eliminated.
7. Very thin cross sections to the order of 0.75 mm can be
8. Die castings can be replaced when short ruins are
9. Castings are sound and have large grains as the rate of
cooling is slow.
10. It represents the only method suitable for manufacture
of precision shaped castings of high melting point
metals which could cause too rapid die failures in
normal die process.
1. It is an expensive process and hence employed only
where small no of intricate and highly accurate parts
particularly high melting point alloys are to be
2. This process is suitable for small size parts
3. This presents some difficulty where cores has to be
The advantages of investment casting are:
• Excellent surface finish
• High dimensional accuracy
• Extremely intricate parts are castable
• Almost any metal can be cast
• No flash or parting lines
The main disadvantage is the overall cost.
Some of the reasons for the high cost
include specialized equipment, costly refractories and binders, many operations to make a
mould, a lot of labor is needed and occasional minute defects. However, the cost is still
less than producing the same part by machining from bar stock; for example, gun
manufacturing has moved to investment casting to lower costs of producing pistols.
Investment casting is used in the aerospace and power generation industries to produce
turbine blades with complex shapes or cooling systems.
Blades produced by
investment casting can include single-crystal (SX), directionally solidified (DS), or
conventional equiaxed blades. Investment casting is also widely used by firearms
manufacturers to fabricate firearm receivers, triggers, hammers, and other precision parts
at low cost. Other industries that use standard investment-cast parts include military,
medical, commercial and automotiv